**HAL Id: hal-01737079**

**https://hal-mines-albi.archives-ouvertes.fr/hal-01737079**

### Submitted on 18 Apr 2018

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**kinematic fields in Ti-6Al-4V serrated chip formation at**

**micro-scale**

### Mahmoud Harzallah, Thomas Pottier, Rémi Gilblas, Yann Landon, Michel

### Mousseigne, Johanna Senatore

**To cite this version:**

### Mahmoud Harzallah, Thomas Pottier, Rémi Gilblas, Yann Landon, Michel Mousseigne, et al.. A

### coupled in-situ measurement of temperature and kinematic fields in Ti-6Al-4V serrated chip

### for-mation at micro-scale. International Journal of Machine Tools and Manufacture, Elsevier, 2018,

### �10.1016/j.ijmachtools.2018.03.003�. �hal-01737079�

## A coupled in-situ measurement of temperature and

## kinematic fields in Ti-6Al-4V serrated chip

## formation at micro-scale

### M. Harzallah

a_{, T. Pottier}

a∗_{, R. Gilblas}

a_{, Y. Landon}

b_{, M. Mousseigne}

b_{, J. Senatore}

b
a Institut Cl´ement Ader (ICA), Universit´e de Toulouse, CNRS, Mines Albi, UPS, INSA, ISAE-SUPAERO, Campus Jarlard, 81013 Albi CT Cedex 09, France
b Institut Cl´ement Ader (ICA), Universit´e de Toulouse, CNRS, Mines Albi, UPS, INSA, ISAE-SUPAERO, 3 rue Caroline Aigle, 31400 Toulouse, France
Keywords

Primary shear zone Digital image correlation Infrared Thermography micro scale

Fast imaging

Abstract

The present paper describes and uses a novel bi-spectral imaging apparatus ded-icated to the simultaneaous measurement of kinematic and thermal fields in or-thogonal cutting experiment. Based on wavelength splitting, this device is used to image small scale phenomenon (about 500×500µm area) involved in the gener-ation of serrated chips from Ti-6Al-4V titanium alloy. Small to moderate cutting speeds are investigated at 6000 images per second for visible spectrum and 600 images per second for infrared measuresments. It allows to obtain unblurred im-ages. A specific attention is paid to calibration issue including optical distortion correction, thermal calibration and data mapping. A complex post-processing procedure based on DIC and direct solution of the heat diffusion equation is de-tailed in order to obtain strain, strain-rate, temperature and dissipation fields from raw data in a finite strains framework. Finally a discussion is addressed and closely analyzes the obtained results in order to improve the understanding of the segment generation problem from a kinemtatic standpoint but also for the first time from an energetic standpoint.

### Introduction

The constant interest in understanding and mastering the ma-chining processes has led researchers to focus more and more closely on the cutting phenomeon. In recent years, various modelling attemps has met with the need of reliable mea-surements to either discriminate and/or validate models [37]. The use of post-mortem analysis such as chip morphology and SEM analysis [57,67,17,61,60] remains the most com-mon approach. Force components measurement in real time trough Kistler dynamometer is also very popular and has be-come almost dogmatic in machining research [53, 33]. Tem-perature measurement using thermo-couples inserted either in the part or in the tool insert has also been investegated to reg-ister macro scale heat generation [24]. The use of such global quantities (chip morphology, cutting force and tool tempera-ture) has proven worthy but limits the understanding of local phenomena such as strain distribution and temperature gen-eration.

To overcome this very issue, some studies have been ded-icated to the assessement of in-situ measurement of thermo-mechanical quantities. The use of Quick Stop Devices has been widely developped in the machining field with some in-tresting results [12,34,30]. More recently, full-field measure-ment techniques have been successfully implemeasure-mented for ma-chining purpose. They offer a real-time and in-situ insight of the thermomechanical fields through surface measurements. Such data exhibit of course a different nature from those

within the bulk of the material but remain valuable either for phenomena understanding or for model validation. Per-forming full-field measurements of any nature in cutting con-ditions exhibits two major difficulies i) the size of the observed area and ii) the rapidity with which the phenomenon occurs. These papers can be sorted in two main categories: strains measurements and infrared (IR) temperature measurements.

Though strain measurements at micro-scale are well doc-umented in a SEM environnement [27, 21, 52], the speed requirement in cutting condition has prevented researchers to adopt this approach to obtain experimental data. Few studies have focused on such measurement, in quasi-static or dynamic conditions, through optical microscopy [29, 42]. Indeed, optical microscopy can easily be coupled with high speed imaging and thus offer a way to work around the two difficulties mentioned in the above. The use of Digi-tal Image Correlation (DIC) has enabled the computation of strains and strain rates at microscale and low cutting speed (Vc = 6.10−4m.min−1) along continuous chips in [13] and at

higher speed (Vc= 6 m.min−1) in serrated chips in [15, 44].

Nevertheless, this technique requires unblurred images and is thus often used at low-to-moderate cutting speed. At higher cutting speed, Particle Image Velocimetry (PIV) is of-ten preferred eventhough it cannot be used for serrated chips [19, 23, 22]. One noticeable exception is the work of Hijazi and Madhavan [28] which have developed a complex dedi-cated device composed of four non-intensified digital cameras set in dual frame mode to perform a 4 unblurred images

ac-∗_{Tel. +33 (0)5 63 49 30 48}

e-mail: thomas.pottier@mines-albi.fr www.institut-clement-ader.org

quisition at 1 MHz and thus use DIC to retreive strains. More recently, the improvement of high-speed camera spatial res-olution enable Baizeau et al. [6] to perform DIC at higher cutting speed (Vc = 90 m.min−1) , this work is not directly

focused on the chip formation but rather on residual stresses in the generated surface and is thus performed at a lower magnification.

Temperature measurement at tool tip within the infrared waveband have been investigated in the early 2000’s by var-ious works includig the pioneer work of [47] which uses IR pyrometry. However, thermographical studies are very sel-dom at high magnification. The completion of thermal mea-surments by corresponding kinematic measures at the same location has been adressed at micro scale by Bodelot et al. [8] with a spatial resolution of 21µm/pixel for the IR frames. The work of Arrazola et al. in [3, 2] also presents thermal measurement in the mid-wave IR band (3 − 5µm) using a home developped IR-microscope. It allowed the measurement of temperature fields with a resolution of 10µm/pixel and an exposure time of 2ms, at a cutting speed of 400m/min. Oth-ers authors have developed various experimental apparatus to obtain temperature fields at high cutting speeds (above 100m.min−1) for continuous chips [54,18,32,59,5]. At such cutting speed, the scale of the problem imposes to use high exposure time, therefore, the obtained images are blurred (time-convoluted) and can thus only be processed when a thermal steady state is reached. The simultaneous measure-ments of strains and temperatures through the same optical path have been first performed by [4, 63]. The authors use Schwarzschild reflective optics to acheive a 15X magnifica-tion and a cold mirror reflects the visible light to a visible camera and transmits infrared light to a mid-wave thermal camera. More recently Zhang et al. [66] have proposed a dual camera measurement of serrated chip generation using a two side configuration. This technique, well known for ten-sile tests proposes to capture visible images on one side of the sample and IR-fields on the other side. Authors acheive the acquisiton of thermal images at 60Hz with a spatial res-olution of 25µm/pix. Accordingly, only small cutting speed 2−4m/min are investigated. Finally the work of [26] presents thermal measurement at very small intergation time (10µs) and 700Hz in the midwave IR band, this allows to obtain unblurred and transient thermal images with a resolution of 33µm/pix and a cutting speed up to 100m.min−1.

### 1

### Experimental Setup

### 1.1

### Orthogonal cutting apparatus

Tests are performed in othogonal cutting configuration using a dedicated device made of a fixed tool and a linear actuator. This latter is fixed on the working plate of a conventionnal milling maching while the tool is fixed on the spindle head (see Fig.1). The feed is set to f = 250µm using the Z-axis wheel. The chosen cutting tools are made from uncoated car-bide and exhibit a rake angles of 0◦. The depth of cut is d = 2.7mm, the length cut is 120mm and the cutting speeds are ranging from 3m.min−1 to 15m.min−1. The typical ge-ometry of the segments generated at these two cutting speeds is depicted in Fig.2d. The three components of the cutting force are recorded through a Kistler dynamometer.

### 1.2

### Imaging apparatus

The proposed imaging device is inspired by the one presented in [4]. The key feature being a spectral separation of the incoming flux though a cold mirror that enables imaging at two different wavelengths, one dedicated to visible images (for DIC purpose) and the other to IR images (temperature mea-surments). The chosen configuration is slightly different in the present paper since the IR flux is here focused by reflec-tion along the optical path. An off-axis parabolic mirror is used instead of a germanium tube lens thus preventing from chromatism throughout the IR spectrum (0.9µm − 20µm).

Lighting is performed from two high power LEDs (1040lm) one is embedded in the imaging system and pro-vide diffuse axial illumination, the other is set outside and is focused directly on the sample thus providing a directional illumination. This latter is also added a low-pass filter to prevent stray IR illumination.

The camera on the visible optical path is a Photron Fast-cam SA3 set at 6000f ps and an exposure time of 25µs. The image resolution is 512 × 512 pixels.

The dimensioning of the thermographic line depends on the expected thermal range. Recent works, in the field of orthogonal cutting [5, 59], with different cutting conditions (speed, angle and material), provides a glance at the expected temperature range of Tmin= 200◦C to Tmax= 550◦C. In

or-der to choose the most suited detector, it is classical to refer to the cross-checking of Planck’s laws calculated at the two extremes temperatures of the range (Eq.1). Indeed, for a blackbody at a given temperature, 95% of the emitted flux is between 0.5λmax and 5λmax, where λmax is provided by

Wien’s displacement law. λ1= 0.5 2898 Tmin λ2= 5 2898 Tmax (1)

Therefore, the optimal spectral band for this temperature range is [3.1 − 17.6]µm. The commercially available detector offers wavelength range of [3 − 5]µm for InSb or MCT detec-tors (Mid-Wave IR) or [8 − 12]µm for microbolometer. In the present paper, the ability of Mid-Wave IR cameras to reach higher acquisition rates, up to 9 kHz with sub-windowing mode, have led to consider this latter type of detector.

Accordingly, the camera on the IR optical path is a FLIR SC7000 set at 600f ps and an exposure time of 50µs. The de-tector is sub-windowed at 1/4 in order to increase the amount of frames per second. It receives radiations through the 1mm-thick silicon beam-splitter of which the measured average transmittance is Tλ≈ 0.66 for wavelengths ranging from 3µm

to 5µm. The IR-image resolution is 160 × 128 pixels.

### 1.3

### Material and samples

The studied material is Ti-6Al-4V titanium alloy, it presents two advantages in the scope of this study: it is industri-ally machined at relatively low cutting speed (typ. below 60m.min−1) and it is known to generate serrated chips even at very low cutting speed [44]. This latter feature being re-lated to the poor thermal conductivity of titanium alloys (typ. below 10 W.m−1.K−1). The microstruture has been investi-gated through SEM and exhibits almost equiax grains with an average size of 19.2µm. The observed surface of the sample

### IR Camera

### CMOS high speed Camera

### Si splitter

### beam splitter

50R/50T### off-axis parabolic

### miror

### power LED

+ focus### Schwarzschild

### objective

### tube lens

### VIS optical path

### IR optical path

### Sample

### Linear

### accuator

### Tool

### Kistler

dynamometer### Conventional

### milling

### machine

### Sample

### holder

Figure 1: a)Orthogonal cutting device and imaging apparatus. b) Schematic of the VIS-IR imaging apparatus

is polished and etched to exhibit microstructure, this matter being used as a natural speckle for DIC (Fig.2a-b).

With such surface treatment, the spectral emisivity of the sample is measured from Fourier transform infrared spec-troscopy. The emissivity spectrum is depicted in Fig.2c. The spectral emissivity λ is here assumed to equal its average

value over the wavelentgh range of the camera denoted . It is also assumed to remain constant within the considered temperature range [20].

The mass density ρ, the specific heat Cpand the thermal

conductivity k are functions of the temperature. According to [7, 9], they are chosen to evolve linearly in-between the boundaries given in Tab.1.

### 2

### Calibrations and optical

### caracter-izations

### 2.1

### Metric calibration

The size of the observed area and the amount of optical trans-mission from object to detectors leads to question either the exact magnification of the apparatus and the possible distor-tions along both visible and IR optical paths.

For magnification assessement purpose, images of cali-brated lines (50 lpm and 31.25 lpm) were captured by both cameras (see Fig. 3a-d). Then a Fast Fourrier Trans-form of the image provide the pixel period of the pattern which lead to a metric ratio of 1.133µm/pixel for the visible camera (Photron Fastcam SA3) and knowing that the pixel pitch of this camera is 17µm, the obtained magnification is Mvis≈ 15.00. The same procedure applied to the IR optical

path leads to a metric ratio of 1.981µm/pixel and a magifi-cation of MIR≈ 15.14 (detector pitch ≈ 30µm).

### 2.2

### Distortions correction

For distortion purpose, image pairs exhibiting rigid body mo-tion along X and Y axis (the horizontal and vertical axis

of the image frame respectively) are captured by both cam-era. The sample is being translated using a two-axis mi-crometric translation stages for a prescribed translation of upres

x = 50µm, then upresy = 50µm. DIC is then performed

between these images in order to assess the imposed displace-ment such that:

( δx(X) = umeasx (X) − u pres x δy(X) = umeasy (X) − u pres y (2)

where δx(X) and δy(X) are the components of the

disor-tion field. Thus, assuming that optical distordisor-tions are zero at the center of the image (δx(0, 0) = δy(0, 0) = 0), the value of

the constant upres can be assessed and the distortions

esti-mated. Fig.3b-e reads the shape and magnitude of δx(X) and

δy(X) for both visible and infrared imaging. Finally, these

noised distortion fields are approximated through the model
presented in [62] and used for DIC purpose in [43]. This
latter proposes to approximate the distortions through the
correction of radial, decentering and prismatic components
as follows:
(_{˜}
δx(X) = x r1ρ2+ r2ρ4+ r3ρ6 + 2d1xy + d2 3x2+ y2 + p1ρ
˜
δy(X) = y r1ρ2+ r2ρ4+ r3ρ6 + 2d2xy + d1 x2+ 3y2 + p2ρ
(3)
where ρ =px2_{+ y}2 _{is the distance to the optical center.}

A simplex optimization algorithm is used to estimate the six parameters of each model and resulting distortion fields are depicted in Fig.3c-f. It can be seen that the optical distor-tions exhibit similar order of magnitude for the two imaging wavelengths although the mirrors alignements issues lead to different shapes of the distortion fields. All subsequent dis-placement and temperature measures presented in this paper are corrected accordingly.

### 2.3

### Image and speckle quality

No special treatment is applied on the sample surface, and the visible microstructure is used as a spekle for the DIC

### (a)

### (b)

### (d)

2.5 3 3.5 4 4.5 5 5.5 0 0.5 1### Wavelength (in µm)

### Spectral Emissivity

### 𝜖

λ### (c)

### 3m/min

500µm### 15m/min

500µmFigure 2: (a) SEM image of a typical Ti-6Al-4V equiax microstructure. (b) Microstructure as-seen from the visible imaging line. The texture is used as a speckle for DIC. (c) Mid-wave infrared emmission spectrum of the sample surface. (d) Typical chip geometry obtained at 3m.min−1 and 15m.min−1.

ρ Cp k

kg · m−3 − J · kg−1· K−1 _{W · m}−1_{· K}−1

20◦C 4450 0.37 560 6.7

550◦C 4392 0.37 750 9.7

Table 1: Chosen material parameters for Ti-6Al-4V [7,9,20].

### a)

### V

### is

### ib

### le

### IR

### 50 lpm target

### c)

### e)

### 31.25 lpm target

### 512x512

### frame

### 160x128

### frame

### b)

### d)

### f)

Figure 3: a) and b) Visible and infrared images of calibrated targets of 50 lines per millimeter(lpm) and 31.25 lpm. c) and d) Shapes and magnitudes (in pixel) of the measured distortion fields along x and y axis for the visible and IR optical path. e) and f ) Approximation of the distortion fileds from the model presented in (Eq.3). Results in pixel.

algorithm. Estimating the measurement uncertainties of speckle related DIC techniques, is known to be a complex task [10, 40]. Lots of studies have been addressed in this field and the point of the present paper is not to discuss any further in this matter. Hence two estimation approaches are here adressed in order to assess the most suited subset size.

The first approach tested here is the so-called Mean Inten-sity Gradient [39], it provides an estimation of displacement precision (standard deviation). In the present work the image MIG is δf = 10.52, the measurement noise is assessed from

the substraction of two motionless images and its standard deviation equals σ = 3.53 pix. Hence the standard deviation of the displacement can be approximated from:

std(u) ≈ √

2σ n ∗ δf

(4)

where n is the subset size (in pixel). Hence, assuming a cho-sen subset size of 16×16 pix, the expected standard deviation of the measured displacements is about 0.03 pix.

The second approach is the use of rigid body motion such as detailed in [56]. This approach is close to the one used in section 2.2. Two images exhibiting a translation motion are captured and displacement are computed and compared to the imposed one. It allows assessing both precision (random error) and accuracy (systematic errors) though this latter re-quires to know the accuracy of the translation stage. For this reason, only the random error is here estimated and equals 0.035 pix for a subset size of 16 × 16 pix. The two approaches provides approximatively the same magnitude of the disper-sion. Hence, cumulating such error over 50 images lead to an maximal error or 1.5 pix and therefore lead to errors on strain below 10% (if a 16 × 16 pix extensiometric basis is used).

### 2.4

### Thermal calibration

Small scale calibration of IR cameras remains a challenging task for the thermography community. Either a specific lens is designed for microscopic observation, and calibration is then classical [49], or the camera is used without lens and the in-coming radiation is focused on the detector array [31]. How-ever, the approach presented in this latter work performs the calibration of the thermal flux ratio at two different wave-lengths (bichromatic thermography), not an absolute one. In the present paper, among the two imaging paths, only one is in the infrared spectrum and thus prevents from the use of the bichromatic approach. The goal is then to perform an accurate thermal calibration (with the smallest interpolation error), at small scale. To do so, several precautions must be respected.

First of all, and as each pixel exhibits a different spectral and electronical response than its neighbours, a Non Unifor-mity Correction (NUC) is necessary. The method used in this paper is the Two Point Correction (TPC), which classically corrects the offsets φ and gains K of each pixel of coordinate X on the average response over every pixels. The relation be-tween the output current of a given pixel and the read digital level is given by

Id(X, T ) = K(X)Icurrent(X, T ) + φ(X) (5)

For calibration sake, two input images are required: a dark and a bright image. They are obtained by placing an integrating sphere (Optronics Laboratories OL400) in front

of the camera and adjusting the lamp supplying current (see Fig.4a).

The second step of the calibration procedure is the ther-mal calibration. This step consists in visualizing a blackbody at different temperatures with the camera, and to choose and parametrize a model which best fits the experimental points (digital level versus temperature). The chosen model is the so-called effective extended wavelength model proposed by [51], which is recalled hereafter :

Id0(T ) = Kwexp − C2 λxT with 1 λx = a0+ a1 T + a2 T2 (6) where I0

d(T ) is the averaged signal provided by the pixels

viewing the blackbody at a temperature T . Kw, and the ai

are the radiometric parameters. Then the parameters identi-fication is performed through the use of a black body set at 10 temperatures Ti ranging from 20◦C to 550◦C (Fig.5b):

log I_{d}0(Ti) = log (Kw) −
C2a0
Ti
−C2a1
T2
i
−C2a2
T3
i
(7)

At small scales, an important source of error is the Size of Source Effect (SSE), which includes the illumination of the detector array by stray light and detector overwhelming [64]. It is then necessary to install a pinhole between the black body and the camera. The obtained image with a 200µm pinhole is depicted in Fig.4b, only the illuminated pixels are used for calibration. It is also verified with other pinholes (100µm and 50µm) that the incoming flux is no longer af-fected below 200µm.

A 3rd _{degree polynomial fit is then used to assess the }

ra-diometric parameters (error to the black body measurement are depicted in Fig.5c). The absolute error is always inferior to 7◦C, and is higher for low temperatures, where the detec-tivity of the pixels becomes very low (i.e. the photoresponse versus the flux of each pixels behaves non-linearly).

Once the calibration performed, in the measurement step, the emissivity must be known to infer true temperature, as defined in the following equation :

(T ) = Id(T ) I0

d(T )

⇒ I_{d}0(T ) = Id(T )

(T ) (8) Combining Eq.(7) and Eq.(8) then gives

log Id(T ) (T ) − log (Kw) + C2a0 T + C2a1 T2 + C2a2 T3 = 0 (9)

where (T ) = is assumed to be constant over the consid-ered temperature range [20]. The computation of the true temperature T at each pixel from the measured intensity Id(T ) is obtained by solving this latter equation. In

prac-tice, this is performed through the Cardano’s method.

### 3

### Measurement Post-processing

### 3.1

### Digital Image Correlation

The DIC computations has been performed with 7D soft-ware [58]. The quality of the obtained images have led to consider the use of incremental correlation [41, 55]. This choice relies on several considerations: very significant strains, microstructure transformation, out-of-plane motion, material decohesion and changing lighting (disorientation). Therefore, the likeness of image no.1 and n is poor and prevent from a

### b)

### a)

### Intergrating Sphere

### IR camera

### Optical Apparatus

### 200µm

Figure 4: a) NUC correction using integrating sphere setup. b) Infrared image of the blackbody at 300◦C through a 200µm pinhole (image at full frame 320 × 256 pixels).

0 100 200 300 400 500 600 0 500 1500 2000 2500 3000 3500

### Black Body Temperature (in °C)

0 1 2 3 4 5 6 7 8 0 100 200 300 400 500 600

### Black Body Temperature (in °C)

### Model

### er

### ror

### (

### in

### °

### C)

ti=50µs### Id

(DI G IT A L L E V E L )### Black Body

### Pin Hole Aperture

### IR Camera

### Optical Apparatus

1000 measures model### a)

### b)

### c)

Figure 5: a) Experimental setup for black body measurement. b) Camera signal as a function of blackbody temperature and
correponding fit. c) Fit error of the black body measurements I_{d}measured− I_{d}f it.

straight forward use of classical DIC. The matching of image n − 1 and n is obtained with better results than images no.1 and n. The counterpart is that such incremental approach re-quires serveral numerical processings in order to compute the cumulated displacements and strains. Fig.6 depicts the res-olution scheme used to retreive global displacement. Indeed, in such resolution scheme, the incremental displacements ∆uk

are obtained (in pixel) at nodes of the correlation grid so that:

∆uk(Xk) (10)

where Xk = (X, Y )k are the correlation grid coordinates

(identical for every image in the image coordinate system but different in the local coordinate system), k being the image number. Accordingly, X0 = x0 = (X, Y )0 is the intial

co-ordinates of the tracked points. This only information does not enable the estimation of strains (whether in initial or fi-nal configuration) since material tracking can not be achieved, cumulating strain and different location is just not right. The evaluation of the deformed coordinates xk = (x, y)k at every

step/images of the deformation process is performed incre-mentally through triangular bi-cubic interpolation.

xk= xk−1+ ∆uk(xk−1) (11) with ∆uk(xk−1) = 3 X i=1 φi(xk−1) × ∆uk(Xk) (12)

where the φiare classical triangular cubic shape functions.

Finally the total cumulated displacement is then obtained as:

uk(xk) = xk− X0 (13)

### 3.2

### Strain Computation

The point of the present experiment is to offer a straight forward comparison of the local mechanical fields between experimental conditions and numerical simulations. For this purpose, strain fields are computed from the observed dis-placements. In a finite strain framework the polar decompo-sition of the strain gradient tensor at instant k states

F = RU = VR (14)

where R is the rotation matrix, and U and V are sym-metric matrices describing the deformations. In most finite element softwares, explicit solvers return various measures of strains. However Eulerian strains such as the Hencky’s strain H (a.k.a. logarithmic strain) or the so-called Swainger’s strain N (a.k.a. nominal strains) are usually prefered in such configuration [1]. Hence, experimental strain measures are obtained from:

H = lnV and N = V − I (15)

where I stands for the identity matrix. The computation of the strain gradient tensor thus becomes the only prerequi-site for strains assessement and is performed from

Fk= ∇X0uk+ I (16)

The space derivative in (Eq.16) leads to a significant issue in experimental conditions: the presence of noise on the mea-sure of uk. In order to address this issue, a filtering method

should be applied on uk prior to any calculation. For this

purpose, a modal projection approach is chosen such as de-scribed in [45] and allows to approximate the displacement by: uk(X0) ≈ N X p=1 αxpQp(X0) , N X p=1 αypQp(X0) ! (17)

where the Qp(X) are the N first eigen modes of a shell

square plate. The αp are the corresponding modal

coordi-nates. The gradient then reads:

∇X0u(X0) ≈ PN p=1αxp ∂Qp(X0) ∂X PN p=1αxp ∂Qp(X0) ∂Y PN p=1αyp ∂Qp(X0) ∂X PN p=1αyp ∂Qp(X0) ∂Y ! (18) Finally, interpolation is used again to obtain the displace-ment gradient, and thus the strains over the deformed grid xk as

∇X0uk(xk) = ∇X0uk(X0+ uk(X0)) (19)

### 3.3

### Thermal imaging post-treatment

The measurement of surface temperature as such is of limited
interest since it has to be matched with the generated powers
involved in the cutting phenomenon. Indeed, as pointed by
many authors [36,24] most of the generated heat is extracted
along with the chip. It therefore affects the cutting force
but only very remotely the generated surface. Accordingly,
the thermal information is mostly intresting from an energy
balance point of view and in order to investigate the tight
couplings between constitutive equations and temperature.
Let’s recall the specific form of the heat diffusion equation in
the Lagrangian configuration applied to a 2D thermographic
framework (readers should refer toAppendix Afor detail on
the establishement of such relation and its related
hypothe-sis).
ρCp
∂ ¯θ
∂t + ~v · ~∇¯θ
−k1 ~∇¯θ
2
−k∆2θ+¯
2hθ
d +
2σ
d ( ¯T
4_{−T}4
r) = w
0
ch
(20)
where:

• ¯θ = ¯T (x, t) − T0 is the difference between the current

surface temperature field and the initial state where the temperature T0 is assumed to be homogeneous and

equal to the room temperature.

• ρCp

∂ ¯θ ∂t+ v∇¯θ

is the inertial term that reads the temperature evolution at a given location (x, t). Vari-able v stands for the velocity vector field.

• k1 ~∇¯θ

2

−k∆2θ is the diffusion (Laplace’s) term. Note¯

that∇ is the two dimensionnal gradient and ∆2the

two-dimensionnal Laplace operator. • 2hθ

d + 2σ

d (T
4_{− T}4

r) is the convective and radiative heat

losses over the front and back faces of the sample. σ here stands for the Stefan-Boltzman constant. h is the heat transfer coefficient arbitrary chosen to equal 50W.m−2.K−1 (forced convection) and d is the depth of cut.

### Incremental

### Displacements

### X

_{0}

### =x

_{0 }

### x

1### X1=X

_{0 }DIC

### Δu

_{2}

### (x

_{1}

### )

### interpolated

### x

_{1 }

### x

_{1 }

### x

_{0 }DIC

### Δu

_{2}

### (X

_{1}

### )

### correlation

### Δu

1### (X

0### )

### correlation

### Cumulated

### Displacements

### x

_{2 }

Figure 6: Illustration of the computation scheme used to assess the cumulated displacement from incremental correlation.

• w0

ch = d1is the heat source term and equals the intrinsic

dissipation d1in absence of the thermoelastic couplings

(seeAppendix A).

• The material parameters are then ρ = ρ1θ +ρ0the mass

density, Cp= C1θ + C0 the specific heat, k = k1θ + k0

the thermal conductivity. The values and dependencies of these parameters to temperature are disscused in the above within the section1.3.

The objective is here to compute the left hand side terms from the measured quantities ( ¯T (x, t) and T0) and the

ma-terial parameters in order to provide an estimation of the
involved power in the cutting phenomenon w0_{ch}. In practice,
the computation of the Laplace operator over noisy data
re-quired the use of filtering. The chosen approach relies on the
same projection used for strains (see Eq.17). In addition, the
time derivative requires to evaluate the temperature in a
La-grangian framework while thermography provides it in
Eule-rian configuration. Hence, Motion Compensation Technique
is used to retreive the material evolution of temperature from
the fixed pixel evolution. Such approach is classical nowaday
and is not detail any further here; readers can refer to [50,46]
for more details.

### 4

### Results

### 4.1

### Test at V

c### = 3m.min

−1The captured images consititues a film depicting the genera-tion of 197 segments. Fig.8a presents 5 raw images of one sin-gle segment generation process (segment no.101). In addition it is worth mentionning that no drift of the thermomechani-cal quantities is observed during the cut. A total of 62 visible images and 6 thermal images are captured for this segment. For reading and comparison purpose, images are labelled by their number and the percentage of the segment formation. The first image (0%) being the image where the segment first touches the tool and the last image (100%) being the image exhibiting a displacement of 50µm after the segment being fully formed. It is seen from the raw images and Fig.8b that

a crack continuously propagates along the primary shear band (denoted ZI in the following). Fig.7a depicts the fluctuations

of the cutting force. It can be seen that the cutting force peaks just prior the crack initiation (around 30%) and drops signif-icantly when the crack reaches completion (about 60%). The magnitude of the force fluctuations equals 150 N meaning a tenth of the overall force. The average cutting force over the whole segment formation is Fc = 1611 N . The Fast Fourier

Transform of the force signal provided in Fig.8b show a typi-cal spectrum of a sum of two Gaussian distributions where the main peak matches the segmentation frequency (110 Hz) and the secondary correspond to the oscillations during the early stages of the segment generation (clearly visible in Fig.7a).

It can be seen from the strain depicted in Fig.8c that the three stages process described in [44] is clearly visible. The first two images (prior to 30% progression) show a diffuse deformation within the segment bulk, included in-between 0.3 and 0.8. Latter on, strains slowly converge to a localized zone ahead of the tool tip (clearly visible from 40%). Starting from this stage, strains accumulate in ZI and lead to material

failure. A crack propagates moving away from the tool tip. From image no.49 (80% and subsequent), the segment is fully formed and is extracted. It therefore undergoes rigid body motion and strains accumulation stops.

The strain rate field depicted in Fig.8d is of localized na-ture in the early stages of the process. Strains are accumlated at the same location all along the segment generation process. There is no clear evidence of any motion of the shearing zone conversly to previouly published results [35]. The primary shear zone model seems therefore particularly suited from these obsevations. Indeed, strain is generated by the fact that material particules are geometrically forced through this band and exit it with a strain that almost no longer evolves afterward (Fig.8c).

The temperatures imaging do not prompt any clear lo-calisation within ZI before 60% (i.e. the end of segment

generation). The maximum temperature do not evolves sig-nificantly during the sequence, only ranging from 317◦C to 360◦C. However, the temperature gradient is significant in space. The min/max range within the same image roughly equals 300◦C. Indeed, the main temperature rise seems to

oc-Cutting force fluctuation frequency (in Hz) 0 50 100 Cut tin g f o rc e (in N ) 1550 1600 1650 1700 150 200 250 300 0 0.2 0.4 0.6 0.8 1 0 5 10 15 20 0 20 10 7 5 4 3 F a st F o ur ie r T ra ns fo rm 𝑓 1550 1600 1650 1700 Times (in ms) Segment n Segment n+1

### a

)### b

)Figure 7: a) Fluctuations of the cutting force over the generation of segment n0.101 and no.102 versus time. b) Fast Fourier Transform spectrum of the whoole force signal at Vc = 3m.min−1.

cur during the transit of a material point through the strain rate line (ZI). It is also worth noticing that the maximum

temperature location is not in the direct vicinity of the tool. Such consideration lead to consider that heat generated in ZI

(from plasticity and damage) prevails over the heat generated in the secondary and tertiary shear zone (due to friction over the rake or draft face).

Conversly to temperature, the computed heat source
(Fig.8f) localizes during the early stage of segementation and
almost simultaneously with the strains (depicted in Fig.8c).
The dissipated power evolution also exhibits three stages: at
fisrt, up to image no.6, the dissipated power is low (about
1.7 × 1012 _{W.m}−3_{) and is concentrated close to the tool.}

Then, from a progression in-between 20% to 60%, the dis-sipated power increases within ZI from 2 × 1012 W.m−3 to

3.2 × 1012 _{W.m}−3_{. The source also sligthly progress }

right-ward (i.e. along the shear band from the tool tip to the free surface). Finally, it is seen from image no.49 (80%) that even while the crack propagation is completed, and that strain accumulation stalls, the generated power remains high and peaks around 3.2 × 1012 W.m−3. It is also visible from the first image that when the generation of segment n starts the input mechanical power is split in two locations, the first con-sists in the sliding of the segment n−1 over the segment n and the second is the early stage of generating segment n. Indeed, it is clearly visible that a second source lights up beneath the sliding band and close to the tool tip.

### 4.2

### Test at V

c### = 15m.min

−1At such cutting speed 248 segment are generated and with a frame rate of 6000 F P S the generation of a single segment last 11 images. Fig.9a depicts 5 images spread over the seg-ment no.107 generation process. Comparatively, with a cap-ture frequence of 600 F P S only one thermal image is acquired during the process and corresponds to a 40% progression. For this very reason, the other thermal images presented in Fig.9e are not otained from the investigated segment but from other measured segments but at the same stages of the segmenta-tion progression. For this test, the average cutting force over the whole segment formation equals Fc= 1516 N .

The crack progression differs from the one presented for a cutting speed of 3 m.min−1 (Fig.8b). Indeed, the crack does not progess from 0% to 40% and suddenly propagates almost all the way to the free surface at image no.6 (60%). The

pheneomon therefore seems to be more brutal at high cutting speed. This observation is confirmed by the investigation of the strain field depicted in Fig.9c. Eventhough these latter exhibit the same kind of diffused strain within the segment bulk (about 0.7), the shear localization within ZI appears

later (at 60% instead of 20% or 40%). It is also worth notic-ing that the total strain reached at 80% (i.e. at failure) is 1.5 which is lower than its counterpart at lower cutting speed (1.7).

The strain rates fields exhibit similar features regardless of the cutting speed. Their magnitude obviously increases with the cutting speed but in a linear manner. Indeed, one would expect that multiplying the cutting speed by 5 would increase the strain-rate magnitude by the same ratio, which is almost the case here. Hence, the difference of crack propaga-tion nature is explained by the only fact that strain at failure decreases as the thermomechanical loadings increases.

As expected, the temperature rises higher as the cutting speed increases and reaches a maximum of 548◦C. It is also seen that the localization of the thermal fields is more obvi-ous at such cutting speed even at the very early stages. In addition, it is observed that the maximum temperature de-creases in the early stage of segment generation (between 10% and 20%) then increases again while the crack reaches com-pletion. This could be explained by the fact that the heat source image at 10% actually reads two primary shear zones, the one at the tool tip (which leads to generate the observed segment) and another one, higher along the tool rake face, correponding to the previous segment.

From this perspective, the thermal dissipation fields de-picted in Fig.9f are consistent with the observation made at 3 m.min−1. Indeed, the heat source originates from the sub-surface at the tool tip then spreads and moves rigthward along ZI. It is also noticed that the dissipation band is narrower.

The magnitude of the source however rises question since it appears to be only multiplied by a factor of roughly 3 while the cutting speed and the strain rate are increased by a factor of 5. This leads to conclude that segmentation in ZI (where

the heat source are higher) do not develops at iso-energy. In addition, it is worth noticing that the dissipation prompts at 80% has exactly the same shape and magnitude that image at 0% (not depicted in Fig9). This illustrates the cyclic nature machining under such conditions.

### FastCam 9414

0

### image 13

### image 6

### image 25

### image 42

### image 50

### FastCam 9424

### FastCam 9434

### FastCam 9444

### FastCam 9454

### Essai 039 –

### (3m/min - 0°)

### Feston alpha

0 0.34 0.68 1.7 1.02 1.36T_{max}=317°C T_{max}=329°C T_{max}=347°C T_{max}=360°C

240 1200 480 720 960 360 88 156 224 292 20

### 20%

### 10%

### 40%

### 60%

### 80%

T_{max}=323°C d

_{1}max

_{=2.56 }

_{d}

1max=3.14 d1max=2.95 d1max=3.22

d_{1}max_{=2.57 } 3.2x1012
.64x1012
1.3x1012
1.9x1012
2.6x1012
0
200 µm

### D

_{eq }

### H

_{eq }

### d

_{1 }

### (d)

### (c)

### (b)

### (a)

### (f)

### (e)

### T

(°C) (s-1_{) }(W.m-3

_{)}

Figure 8: a) Raw images of the chosen segment at 3m.min−1, images no.6, no.13, no.25, no.42 and no.50 (final image is no.62). b) Crack evolution along the primary shear zone. c) Logarithmic equivalent strain. d) Equivalent strain rate (in s−1). e) Measured temperature (in◦C). f ) Intrinsic dissipation (specific mechanical power in W.m−3).

### FastCam 3337

0.3 0.6 1100 13 8.2 10.6### image 2

### image 1

### image 4

### image 6

### image 8

### FastCam 3338

### FastCam 3340

### FastCam 3342

### FastCam 3344

### Essai 041 –

### (15m/min - 0°)

### Feston Gamma

### d

_{1 }1.5 0.9 1.2 0.00 5500 2200 3300 4400

### EXACT=120

EXTRAP img 121 (Flir) EXTRAP img 119 (Flir)EXTRAP img 114 (Flir) EXTRAP img 112(Flir)

550 126 232 348 444 20

### 20%

### 10%

### 40%

### 60%

### 80%

d_{1}max

_{=7.94 }

_{d}

1max=9.46 d1max=9.49 d1max=9.04 d1max=8.30

0

T_{max}=541°C T_{max}=507°C T_{max}=505°C T_{max}=533°C

9.5x1012 1.9x1012 3.8x1012 5.7x1012 7.6x1012 0 200 µm

### D

_{eq }

### H

_{eq }

### d

_{1 }

### (d)

### (c)

### (b)

### (a)

### (f)

### (e)

### T

(°C) (s-1_{) }(W.m-3

_{)}T

_{max}=548°C

Figure 9: a) Raw images of the chosen segment at 15m.min−1, images no.1, no.2, no.4, no.6 and no.8 (final image is no.10). b) Crack evolution along the primary shear zone. c) Logarithmic equivalent strain. d) Equivalent strain rate (in s−1). e) Measured temperature (in◦C). f ) Intrinsic dissipation (specific mechanical power in W.m−3).

### 5

### Discussion

The use of coupled measurement provides a valuable insight of serrated chips generation phenomenon from which some conclusions can be drawn but it also rises many subsequent questions. The present disscussion aims at summarizing and sorting the obtained information.

### 5.1

### Force measurements

First, as seen from the heat source assessement, the gener-ation of segment n partially overlap in time the genergener-ation of segments n − 1 and n + 1. This explains the difficulty in post-processing macroscopic measurment such as force mea-surements. Indeed, the variations of the force applied by a segment on the rake face cannot be measured from dynamo-metric measurements since the force applied by segment n sum up with the force applied by segment n + 1 or n − 1 [15]. It is also seen that the overall cutting force decreases as the cutting speed increases (from 1611 N down to 1516 N ). This results is easily explained by the addition of thermal softening (significant between 300◦ and 550◦C [14]) and the stick-slip nature of the friction phenomenon at low cutting speed [65].

### 5.2

### Kinematic fields

Second, eventhough the strain fields are heterogeneous in space and in time, it seems that the strains always cumu-late at the same location. As seen from strain rates field, the straining band is fixed in space and only fluctuates in magnitude over time. In addition, other tests performed with different rake angles (not presented here) suggest that the shape of the straining zone (its angle) is strongly related to the cutting geometry (feed and rake angle). This is clearly a perspective to the present work [25].

The equivalent strain at failure is smaller at high cutting speed eventhough the temperature in ZI is higher. A first

explanation for this phenomenon would be that the loss of ductility due to the viscous behaviour of metal overtakes the thermal softening in this range of thermo-mechanical load-ing. Another explanation would be related to the nature of the strain field itself. Indeed, as seen from the heat sources computations, the primary shear band narrows as strain rate increases which pleads for a strain path closer to pure shear than its counter-part at low cutting speed. This latter expla-nation seems to be confirmed by the detailed results presented in Fig.10 in which it is seen that at small cutting speed, the deformation in ZI is a mix of shear and compression while at

15 m.min−1, shear is clearly the main straining mode.

### 5.3

### Thermal informations

From a thermal stand point, the maximum temperature is always observed within ZI and away from the tool. One

can therefore assumed that the temperature measured from a thermocouple positioned within the insert do not reads the proper temperature of ZI. Consequently, it is hard to

ex-trapolate from such measure the value of τf the shear friction

stress and therefore the generated heat flux along ZII

com-monly defined as [24]:

˙

q = βslηf· τf· Vsl (21)

where Vsl is the sliding velocity and ηf the part of the

frictional work converted into heat. βslis the ratio of the

fric-tional power entering the material (1 − βsl being the power

ratio entering the tool). Indeed, the thermal softening of the material in ZI is the leading factor of the stresses at tool/chip

interface (i.e. ZII) and a proper knowledge of temperature

distribution in ZI is therefore a key issue in assessing any

energetic quantity in ZII.

Although most of the heat ultimately ends up in chip, it is seen that the temperature spreads significantly beneath the tool (i.e. in the generated surface) for both cutting speeds. Further investigations are required to link this heat peak to the residual stresses distribution in the generated surface.

As expected, multiplying the cutting speed by five do not multiply the temperature variation (θ = T (x, t) − T0) by five

but only by 1.5 while the maximum dissipated power within ZI (see Fig.8f and Fig.9f) is roughly multiplied by 3. This

simple observation challenges the adiabaticity hypothesis of-ten set within the three shear zones Zi. If the dissipation is

multiplied by 3, under adiabatic conditions, the temperature variation should by multiplied by 3 as well, which is not the case, meaning that the heat is somehow diffusing. Indeed, it is also observed that the second term (the so-called Laplace’s term) of the heat diffusion equation Eq.(20), is clearly not negligible before the inertial term (ρCpθ) especially at small˙

cutting speed. As seen in Fig.11, at 15m.min−1, these two terms exhibits the same order of magnitude, eventhough the thermal conductivity of titanium allows is small.

### 5.4

### Local Powers

From an energy stand point, it is also noticed in Fig.11, that the convective and radiative thermal losses on the side of the sample are negligible. It is also reasonnable to as-sume that even if extrapolated at higher cutting speeds (typ. 60m.min−1) it remains negligible despite the presence of T4. Alike the thermal losses, the variation of kinetic energy is small and will remain so, regardless of the cutting speed. Un-der such hypothesis and those exposed in Appendix A, the classical power balance becomes (local formulation):

w_{ext}0 = −w_{int}0 + ˙k = w_{e}0 + w0_{a}+ ˙k
⇒ w0

ext≈ w0a

(22)

where w0_{ext}and w_{int}0 are the external and internal specific
power, w_{e}0 and w_{a}0 are the elastic and anelastic powers and ˙k
is the variation of kinetic energy.

Zone I: Heat is mainly generated within ZI. Indeed, at

both cutting speed, the dissipated powers at stake and the temperatures in ZII and ZIII are significantly lower than in

ZI. However, plasticity may not, on it’s own, be responsible

for the observed dissipated power in ZI. Indeed, recalling that

Fig.8f and Fig.9f read the left hand side terms of Eq.(20) and assuming that plasticity is the only phenomenon involved in the thermal rise within ZI, it classically comes that the

spe-cific dissipated power equals [16]:

wch0 = βwa0 = β (σ : ˙p) (23)

where β is the so-called Taylor-Quinney coefficient. Note that the thermo-elastic coupling is here neglected before plas-ticity [11]. Hence, assuming a constant value of β of 0.8 ([38]), it comes that the maximal value of the equivalent Von-Mises stresses roughly equal 2.1 GP a for the test at 15 m.min−1and

-0.8 -0.6 -0.4 -0.2 0 -1 Minor strain Ma jo r str a in

### c)

0.2 0.4 0.6 0.8 1 0 3 m/min image no.42 (60%) 200μm Too l### a)

15 m/min image no.6 (60%) 200μm Current position Former/future positions Too l### b)

Figure 10: a) Trajectory of the considered point, up to material failure, for the test at 3 m.min−1. b) Trajectory of the considered point, up to material failure for the test at 15 m.min−1. c) Strain path up to failure for both considered points (cutting speed) in the strain principal plane.

0 0.8 1.6 2.4 3

### x10

12Inertial term

-1 -0.5 0 0.5 1.5

### x10

8Specific kinetic power

### x10

120 2 4 6

Laplace term

### x10

120 2.3 4.6 6.9 9.2

Specific calorific power

0 0.4 0.8 1.2 1.6

### x10

7Boundary conditions

### W.m

-3_{W.m}

-3 _{W.m}

-3 _{W.m}

-3 _{W.m}

-3
1

Figure 11: Shares of power contribution for the test at 15m.min−1 (progression 40%) unit is W.m−3. a) Inertial term. b) Diffusive (Laplace) term. c)boundary condtion term. d) Intrinsic dissipation. e) Kinetic term.

3.3 GP a for the test at 3 m.min which seems largly over-estimated. Such calculation is, of course, too coarse but lead to consider that, especially at small cutting speed, other phe-nomenon are involved (damage, segment-over-segment fric-tion, phase transifric-tion, recrystalization...) and that other dis-sipative terms should be padded to the right hand side of Eq.(22).

Zones II and III : The presented measurements mainly focused on the primary shear zone. Nonetheless they provide valuable information on other dissipatives zones (namely ZII

and ZIII). Indeed, from the thermal information it is

possi-ble to assess the heat flux transfering between the tool and the material. The Neumann boundary condition provides the incoming surface heat flux which can be compared to Eq.(21) as:

˙

q = −k∂θ

∂x = βslηf· τf· Vsl− h(Tw− Ttool) (24) Hence, evaluating the temperature gradient over the ma-terial frontier ∂Ω provides the heat fluxes depicted in Fig.12

for both ZII and ZIII. It can be seen that the power

gener-ated by friction in ZIIis not sufficient to overcome the natural

flux heading from the hot segment toward the tool (cooler). It is also seen that increasing the cutting speed slightly in-creases the outbound heat flux. However, this increase is not proportional to the cutting speed and is to be matched with the tool temperature (see Eq.(24)). Regarding Eq.(24), it can be concluded that in ZII, the current tool temperature Ttool

is of the utmost importance for whoever wants to relate tool wear to the incoming thermal flux. Indeed, if Ttoolis no longer

an unknown variable, a given set of parameters βsl, ηf and h

leads to a possible assessement of the last unknown variable: τf a key variable in machining operations.

In ZIII heat is entering the material, meaning that the

generated surface is hot and slowly diffuses within the
ma-terial. It is seen that the cutting speed strongly affects the
surface temperature beneath the tool which doubles between
3 m.min−1 _{and 15 m.min}−1 _{(approximatively 140}◦_{C and}

300◦C). This ratio of 2 is also observed between the heat flux in ZIII depicted in Fig.12. No discontinuity is observed

in the incoming flux which leads to consider that there is no contact between the tool and the part along the clearance face.

### 5.5

### Global Powers

From a global stand point, it is worth recalling that the overall input power of the cut is the cross product of the cutting force with the cutting speed and that the internal energy balance alows to write that:

Wext0 = Fc· Vc = −Wint0 + ˙K = We0+ Wa0+ ˙K (25)

where ˙K is the variation of kinetic energy, W_{int}0 is the
in-ternal power, W_{e}0 the elastic power, W_{a}0 the anelastic power,
all being expressed in W atts. Hence, by neglecting the
elas-tic power and ˙K before the anelastic power, it is possible to
evaluate the part of energy consumed in each of the three
zones from the spatial intergation of the specific dissipation
w0_{ch}= βw0_{a} depicted in Fig.8f and Fig.9f. It therefore comes:

Wext0 = d β Z SIV i=IZi w0chdS (26)

where d is the depth of cut, Zi is the surface area of the

zones ZI, ZII and ZIII and ZIV is the remaining surface

cor-responding to the imaged sub-surface of the sample and the bulk of the chip segment as depicted in Fig.13. The volume integration is performed under the strong assumption that the heat source is of homogeneous nature along the depth of the sample. Finally, dividing this quantity by the cutting speed results in obtaining ˜Wext expressed in J.m−1; the

en-ergy required to perform 1 meter of cut. Fig.13 depicts for the 5 instants of each tests, the shares of energy consumed by each of the three zones (ZI, ZII, ZIII) and in the rest of

the imaged area ZIV (denoted bulk & sub-surface in Fig.13).

Various considerations can be made from such representation: • As expected from the force measurements interpreta-tion, the overall consumed energy decreases as the cut-ting speed increases (which is consistant with classical dynamometric observation).

• The dissipation in the segment bulk and in the sub-surface (i.e. outside of the three indentified and well known shear zones) is far from negligible. It is con-sistent with the strains measurments presented in the above where it is seen that smaller but significant de-formation occurs within the bulk of the segment. • The dissipation in the segment bulk suddenly drops

when the crack propagation reaches completion (see Fig.13progression 60% for both tests).

• The energy dissipated through plasticity in the sub-surface of ZII and ZIII slightly increases with the

cut-ting speed, especially for ZIII. The interpretation of

(Eq.23) leads to assume that the plastic deformation in these zones also increases with the cutting speed. • For most of the investigated instants, the internal

en-ergy comes close to the external one. Meaning that most of the energy is used within the captured area. How-ever, a part of the input energy is consumed outside of the image. Further investigations would be required to sort out if this energy is used to deform the subsurface (left of ZIII) or the top section of ZI both unseen from

the imaging apparatus.

### Conclusions and Perspectives

In this paper, the development and the implementation of an original imaging apparatus dedicated to the simultaneous measurement of strain and temperature fields at small scale is presented. The proposed experiment enables the monitoring of a 500 × 500µm area at the tool tip using both visible and infrared cameras. The study provides a novel and valuable in-sight to essential thermomechanical couplings and in-process mechanical phenomena involved in the generation of serrated chips and thus gives a new understanding of essential cutting process mechanics occurring during the orthogonal cutting of Ti-6Al-4V. The developed numerical post-processing also constitutes an original contribution since it provides fields information at various time steps of the serrated chip gen-eration progression. Strain, strain-rates, temperatures, dis-sipated powers along with displacement, velocity and crack progression are obtained at each pixel from both kinematic and thermal/energy measurement. It allows the assessment

### 3 m.min

-1 100 µm 100 µm### 0

_{0.5}

### 1

### 1.5

### 2

### 2.5

x107### 15 m.min

-1### 𝑞 (𝑊. 𝑚

−2_{)}

### (b)

### 𝑞 (𝑊. 𝑚

−2_{)}

### (a)

### 3 m.min

-1Figure 12: Averages heat flux entering/exiting the material from the tool/part interfaces of ZII and ZIII during one segment

generation. a) at 3 m.min−1. b) at 15 m.min−1

of the dissipated powers at stake during material removing processes. The whole measuring chain has been strongly cal-ibrated and a special attention has been paid to the depen-dency of the physical parameters to temperature.

The experimental observations have highlighted the de-pendency of the physical phenomena to the cutting speed. This work provides valuable experimental evidences on the different nature of the coupling phenomenon. First, it appears that the nature of the deformation mechanisms is clearly af-fected by the cutting speed, in terms of magnitude but also in term of strain path. At low cutting speed, the loading in the primary shear zone is a mix of shear and compression, while it becomes mainly pure shear at higher cutting speed. Also, the width of the primary shear zone decreases as the cut-ting speed increases. It has been confirmed that the heat is mainly generated in the primary shear zone, and the highest temperature is observed in this zone and not along the rake face interface. In addition, the energetic study conducted in this work demonstrated that the adiabaticity hypothesis of-ten set within the three shear zones is disputed. Indeed, as the dissipation is multiplied by 3, the temperature variation is not multiplied by 3 as well, meaning that the heat is some-how diffusing. It is also observed that the Laplace’s term of the heat diffusion equation is clearly not negligible before the inertial term, especially at small cutting speed. Moreover, plasticity is not the only responsible for the dissipated power in the primary shear zone. Other phenomena may be involved (damage, segment-over-segment friction, phase transition, re-crystallization...). The study also showed that a significant power is dissipated outside the three shear zones and mostly within the segment bulk.

Moreover, even though the heat is mainly evacuated within the chip, the generated surface temperature evolution is significant and this surface is most probably thermally af-fected. This constitutes a direct perspective of this work. A proper knowledge of temperature distribution in this zone is a key issue in assessing any energetic quantity in the chip, in the material and at the tool/chip interface. Especially, acquiring detailed coupled measurements in ZII and ZIII would be of

high interest in order to improve understanding of tool wear and of the thermal influence on the fatigue behavior of the

generated surface.

### Appendix A

Let’s assume a thermal dependance of the physical constants: thermal conductivity, mass density and specific heat as

k = k(θ) = k1θ(x, t) + k0 ρ = ρ(θ) = ρ1θ(x, t) + ρ0 Cp= Cp(θ) = C1θ(x, t) + C0 (27)

where k1is the first term of the linear regression from the

data presented in Tab.1 and k0 the thermal conductivity at

20◦C (idem for the ρi and Ci). θ = T (x, t) − T0(x) is the

temperature variation to the initial temperature T0 The heat

diffusion equation with variable conductivity, mass density and specific heat is:

ρCp

dθ dt − ~∇

k ~∇θ= w0_{ch}+ r(θ) (28)

where w0_{ch} is the specific calorific power (i.e. the internal
heat source).The thermoealstic coupling are here neglected
since the plastic strains largely prevail over the elastic ones.
Readers can refer to [11] and [48] for more details. Another
hypothsesis assumed here is that r, the volume external

ra-diative sources do not depend on temperature T . It comes that r(T ) = r(T0) and therefore that r(θ) = 0.

Using the Kirshoff transform of the temperature:

Ψ(T ) = Z θ

0

k(θ0)dθ0 (29)

and its two subsequent relations dΨ dt = k dθ dt and ~ ∇Ψ = k~∇θ (30)

the heat diffusion equation Eq.(28) becomes:
ρCp
k
dΨ
dt
| {z }
I(Ψ)
− ~∇ ~∇Ψ
| {z }
D(Ψ)
= w0_{ch} (31)

where the left hand side term I(Ψ) is called the inertial term and the right one D(Ψ) is called diffusive term.

10% 20% 40% 60% 80% 0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6

### Progression

### M

### ec

### h

### a

### n

### ica

### l

### en

### er

### g

### y

### (in

### k

### J

### .m

-1### )

1.8 Average 0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6### M

### ec

### h

### a

### n

### ica

### l

### en

### er

### g

### y

### (in

### k

### J

### .m

-1### )

1.8### a)

### Z

_{III }

### TO

### O

### L

### Z

II### Z

IV (chip bulk)### Z

_{III}

### Z

II### Z

I ext### 3 m.min

-1### 15 m.min

-1### b)

### c)

### Imaged

### zone

Figure 13: Shares of energy consumed per zone of the image (red dot stand for the external energy ˜Wext).a) at 3 m.min−1

The key point here is that the available experimental data do not read the third dimension of the temperature fileds (along z). Indeed the thermal information is of surface na-ture and therefore requires to integrate the relation Eq.(31) over the z direction (through-thickness dimension). for this purpose the through thickness average of fields varaibles must be defined as: ¯ • = 1 d Z d 0 •dz (32)

where d is the thickness of the sample (i.e. the depth of cut). This imposes the set two main hypothesis [16]:

i ) The calorific power w0

ch is constant through thickness :

¯ w0

ch= w0ch

ii ) The heat conduction is much greater than the ther-mal losses (radiative and convective) of the front and back faces. It therefore comes that the averaged tem-perature through thickness can be approximated by the measured surface temperature ¯θ ≈ θ(z = 0) ≈ θ(z = d). the integrated diffusive term then becomes:

¯
D = 1
d
Z d
0
∂2_{Ψ}
∂x2 +
∂2Ψ
∂y2 +
∂2Ψ
∂z2
dz
=1
d
∂2
∂x2
Z d
0
Ψdz +1
d
∂2
∂y2
Z d
0
Ψdz +1
d
∂Ψ
∂z
d
0
= ∂
2_{Ψ}_{¯}
∂x2 +
∂2_{Ψ}_{¯}
∂y2
+1
d
k∂θ
∂z
d
0
= ∆2Ψ +¯
1
d
k∂θ
∂z
d
0
(33)

where ∆2is the two-dimensional Laplace operator such as

∆2Ψ = ~¯ ∇ · ~∇ ¯Ψ = ~∇ ·k(¯θ) ~∇¯θ = ~∇ ·k1θ ~¯∇¯θ + k0∇¯~θ = k1∇ · ¯~ θ ~∇¯θ + k0∇ · ~~ ∇¯θ = k1 ~∇¯θ · ~∇¯θ + ~∇ · ~∇¯θ × ¯θ + k0∆2θ¯ = k1 ~∇¯θ2+ ∆¯θ × ¯θ + k0∆2θ¯ = k1 ~∇¯θ 2 + k∆2θ¯ (34)

and ∇ is here the two-dimensional gradient. The integrated inertial term ¯I is expressed through the partial derivative of Ψ and the Liebniz intergration rule as:

¯ I = 1 d Z d 0 ρCp k dΨ dt dz = ρCp kd d dt Z d 0 Ψdz = ρCp k d ¯Ψ dt = ρCp d¯θ dt = ρCp ∂ ¯θ ∂t + ~v · ~∇¯θ (35)

where ~v = ~v(x, t) is the 2D velocity vector field. Finally, it should be noticed that the right hand side term of eq.(33) reads the boundary condition of the front and back faces of the sample. Therefore, assuming a convective/radiative con-ditions on these faces and an room temperature denoted Tr

that equals the intitial temperature T0, one can write that:

− k∂θ ∂z d 0 = 2h¯θ + 2σ( ¯T4− T4 r) (36)

and the completed heat diffusion of the problem at instant t can be expressed as:

ρCp ∂ ¯θ ∂t + ~v · ~∇¯θ − k1 ~∇¯θ 2 − k∆2θ +¯ 2hθ d + . . . 2σ d ( ¯T 4 − Tr4) = w0ch (37) Remark: under such formalism, the use of a Stefan-Boltzmann condition imposes to express the tempratures T and Tr= T0in Kelvin (and not in Celsius)

### References

[1] Abaqus, Inc. ABAQUS Theory guide : version 6.12-1. Providence, RI, USA : ABAQUS, 2016.

[2] J.P. Arrazola, I. Arriola, and M.A. Davies. Analysis of the influence of tool type, coatings, and machinability on the thermal fields in orthogonal machining of AISI 4140 steels. CIRP Annals - Manufacturing Technology, 58:85–88, 2009.

[3] P.J. Arrazola, I. Arriola, M.A. Davies, A.L. Cooke, and B.S. Dutterer. The effect of machinability on thermal fields in orthogonal cutting of aisi 4140 steel. CIRP An-nals - Manufacturing Technology, 57:65–68, 2008. [4] I. Arriola, E. Whitenton, J. Heigel, and P.J. Arrazola.

Relationship between machinability index and in-process parameters during orthogonal cutting of steels. CIRP Annals - Manufacturing Technology, 60:93–96, 2011. [5] J. Artozoul, C. Lescalier, O. Bomont, and D. Dudzinski.

Extended infrared thermography applied to orthogonal cutting. Applied Thermal Engineering, 64:441–452, 2014. [6] T. Baizeau, S. Campocasso, G. Fromentin, F. Rossi, and G. Poulachon. Effect of rake angle on strain field dur-ing orthogonal cuttdur-ing of hardened steel with c-bn tools. Procedia CIRP, 31:166–171, 2015.

[7] D. Basak, R.A. Overfelt, and D. Wang. Measurement of specific heat capacity and electrical resistivity of in-dustrial alloys using pulse heating techniques. Interna-tional Journal of Thermophysics, Vol. 24, No. 6, Novem-ber 2003, 24(6):1721–1733, 2003.

[8] L. Bodelot, E. Charkaluk, L. Sabatier, and P. Dufr´enoy. Experimental study of heterogeneities in strain and tem-perature fields at the microstructural level of polycrys-talline metals through fully-coupled full-field measure-ments by digital image correlation and infrared thermog-raphy. Mechanics of Materials, 43(11):654 – 670, 2011.

[9] M. Boivineau, C. Cagran, D. Doytier, V. Eyraud, M. H. Nadal, B. Wilthan, and G. Pottlacher. Thermophysi-cal properties of solid and liquid ti-6al-4v (ta6v) alloy. International Journal of Thermophysics, 27(2):507–529, 2006.

[10] M. Bornert, F. Br´emand, P. Doumalin, M. Dupr´e, J-C. Fazzini, M. Gr´ediac, F. Hild, S. Mistou, J. Molimard, J-J. Orteu, L. Robert, Y. Surrel, P Vacher, and B. Wat-trisse. Assessment of digital image correlation measure-ment errors: Methodology and results. Experimeasure-mental Me-chanics, 49:353–370, 2008.

[11] T. Boulanger, A. Chrysochoos, C. Mabru, and A. Galtier. Calorimetric analysis of dissipative and ther-moelastic effects associated with the fatigue behavior of steels. International Journal of Fatigue, 26:221–229, 2004.

[12] J. Buda. New methods in the study of plastic deforma-tion in the cutting zone. CIRP Annals, 21:17–18, 1972. [13] S.L. Cai, Y. Chen, G.G. Ye, M.Q. Jiang, Wang H.Y.,

and L.H. Dai. Characterization of the deformation field in large-strain extrusion machining. Journal of Materials Processing Technology, 216:48–58, 2015.

[14] M. Calamaz, D. Coupard, and F. Girot. A new mate-rial model for 2d numerical simulation of serrated chip formation when machining titanium alloy ti-6al-4v. In-ternational Journal of Machine Tools and Manufacture, 48(3-4):275–288, 2008.

[15] M. Calamaz, D. Coupard, and F. Girot. Strain field mea-surement in orthogonal machining of a titanium alloy. Advanced Materials Research, 498:237–242, 2012. [16] A. Chrysochoos and H. Louche. An infrared image

processing to analyse the calorific effects accompanying strain localisation. International Journal of Engineering Science, 38:1759–1788, 2000.

[17] C. Courbon, T. Mabrouki, J. Rech, D. Mazuyer, F. Per-rard, and E. D’Eramo. Further insight into the chip for-mation of ferritic-pearlitic steels: Microstructural evo-lutions and associated thermo-mechanical loadings. In-ternational Journal of Machine Tools & Manufacture, 77:34–46, 2014.

[18] M.A. Davies, A.L. Cooke, and E.R. Larsen. High bandwidth thermal microscopy of machining. CIRP Annals -Manufacturing Technology, 54(1):63–66, 2005.

[19] E.P. Gnanamanickam, S. Lee, J.P. Sullivan, and S. Chan-drasekar. Direct measurement of large-strain deforma-tion fields by particle tracking. Measurement science and technology, 20:095710 (12p), 2009.

[20] L. Gonz´alez-Fern´andez, E. Risue˜no, R.B. P´erez-S´aez, and M.J Tello. Infrared normal spectral emissivity of ti-6al-4v alloy in the 500 - 1150 k temperature range. Journal of Alloys and Compounds, 541:144–149, 2012. [21] A. Guery, F. Hild, F. Latourte, and S. Roux. Slip

activi-ties in polycrystals determined by coupling dic measure-ments with crystal plasticity calculations. International Journal of Plasticity, 81:249–266, 2016.

[22] Y. Guo, M. Efe, W. Moscoso, D. Sagapuram, K.P. Trum-ble, and S. Chandrasekar. Deformation field in large-strain extrusion machining and implications for deforma-tion processing. Scripta Materialia, 66:235–238, 2012.

[23] Y. Guo, C. Saldana, W.D. Compton, and S. Chan-drasekar. Controlling deformation and microstructure on machined surfaces. Acta Materialia, 59:4538–4547, 2011.

[24] B. Haddag, S. Atlati, M. Nouari, and M. Zenasni. Anal-ysis of the heat transfer at the tool-workpiece interface in machining: determination of heat generation and heat transfer coefficients. Heat Mass Transfer, 51:1355–1370, 2015.

[25] M. Harzallah, T. Pottier, J. Senatore, M. Mousseigne, G. Germain, and L. Landon. Numerical and exper-imental investigations of ti-6al-4v chip generation and thermo-mechanical couplings in orthogonal cutting. In-ternational Journal of Mechanical Sciences, 134(Supple-ment C):189 – 202, 2017.

[26] J.C. Heigel, E. Whitenton, B. Lane, M.A. Donmez, V. Madhavan, and W. Moscoso-Kingsley. Infrared mea-surement of the temperature at the tool-chip interface while machining ti-6al-4v. Journal of Materials Process-ing Technology, 243:123–130, 2017.

[27] E. H´eripr´e, M. Dexet, J. Cr´epin, L. G´el´ebart, A. Roos, M. Bornert, and D. Caldemaison. Coupling between ex-perimental measurements and polycrystal finite element calculations for micromechanical study of metallic mate-rials. International Journal of Plasticity, 23:1512–1539, 2007.

[28] A. Hijazi and V. Madhavan. A novel ultra-high speed camera for digital image processing applications. Mea-surement Science and Technology, 19(8):1–11, 2008.

[29] A. I¸c¨oz, L. Patriarca, M. Filippini, and Beretta S. Strain accumulation in tial intermetallics via high-resolution digital image correlation (dic). Procedia Engineering, 74:443–448, 2014.

[30] S.P.F. Jaspers and J. Dautzenberg. Material behaviour in metal cutting: Strains, strain rates and temperatures in chip formation. Journal of Materials Processing Tech-nology, 121:123–135, 2002.

[31] Andrew Justice, Ibrahim Emre Gunduz, and Steven F. Son. Microscopic two-color infrared imaging of nial re-active particles and pellets. Thin Solid Films, 2016. The 43rd International Conference on Metallurgical Coatings and Thin Films.

[32] R.V. Kazban, K.M. Vernaza Pe˜na, and J.J. Mason. Measurements of forces and temperature fields in high-speed machining. Experimental Mechanics, 48(3):307– 317, 2008.

[33] F. Klocke, D. Lung, S. Buchkremer, and I. S. Jawahir. From orthogonal cutting experiments towards easy-to-implement and accurate flow stress data. Materials and Manufacturing Processes, 28(11):1222–1227, 2013.